CHAPTER 3. Si / PEDOT:PSS hetero-interfaces for transparent solar cells
3.3 Results and Discussion
Figure 1a shows the entire manufacturing process of TSC based on a standalone film of n-type SiMW array embedded in poly (dimethyl siloxane) (PDMS). As shown in figure 1b, a hexagonal array of microwires 2 μm in diameter and 30 μm in length was prepared by a photolithography process including reactive ion etching (RIE) using a Cr dot array as an etching mask. Secondly, a 15 nm thick Al 2 O 3 layer is deposited on the SiMW by atomic layer deposition (ALD) to passivate the Si surface. Compared with conventional silicon solar cells, the standalone SiMPF-based TSC in this study has a very high surface area. Therefore, proper surface passivation is essential. As can be seen in Figure 2, TSCs without Al2O3 passivation have very low leakage currents due to surface defects, resulting in very low short circuit current density (Jsc) and open voltage (Voc). Third, SiMW arrays were embedded in PDMS through spin coating. PDMS embedding was performed by a two step spin coating process consisting of a primary spinning for 120 seconds at 600 rpm and a secondary spinning
process for 10 seconds at 1500 rpm. In the first step, PDMS conformally and densely fills the SiMW array. Excess PDMS residue on top of the SiMW was removed during the second spin coating. Al2O3-coated SiMW arrays were found to be hydrophobic enough that PDMS could not penetrate deep into the bottom of SiMW, and the adhesion between SiMW and PDMS was not very strong. Thus, PDMS was easily stripped from the SiMW array in the second spin coating step (Figures 3a and b). The surface of Al2O3-coated SiMW was treated with O2- plasma to improve adhesion between Al2O3 surface and PDMS due to covalent bonding of O- Si [34-36]. Figure 1c shows an SEM image of a SiMW array embedded in a PDMS, where PDMS can be seen deeply penetrating into the bottom of the SiMW array after oxygen plasma treatment. Fourth, the residual PDMS layer was removed by dry etching using a gas mixture of O 2 and SF 6. PDMS can be selectively etched because SFMW is protected by SiMW by an Al2O3 film etched very slowly by SF6 gas. Fifth, the SiMW array embedded in the PDMS was peeled from the Si wafer to generate a flexible standalone SiMW array-PDMS composite film (SiMPF) as shown in figure 1d. As indicated by the hexagonal array of diffraction spots when the SiMPF is illuminated vertically with a 532nm diode laser, the pitch and hexagonal array of the SiMW array was maintained even after peeling off the parent substrate (Figure 4). Finally, the TSC process was completed by forming a hetero p-n junction of indium doped zinc oxide (IZO) ohmic contacts at the bottom of the PEDOT: PSS and SiMPF at the exposed tip.
After changing the pitch defined by the distance between the centers of the microwires from 4 to 7 μm in 1 μm intervals (Figure 6), Figures 6a and b represent the current density (J) -voltage (V)) Characteristics and External Quantum Efficiency (EQE) of TSC Based on Flat SiMW Arrays. A summary of device characteristics is presented in Table 1. In addition, the Jsc, Voc and efficiency of the eight solar cells made with pitch indicate that the box distribution is quite narrow, indicating that this manufacturing process is fairly reproducible as shown in figure 7.
Compared to bulk solar cells, nanowire or microwire solar cells typically have a very large surface area and thus have a high concentration of surface defects that act as leakage current paths [37, 38]. However, the deposited Al2O3 layer has a very low density of interface defects [39-41]. Therefore, surface defects and dangling bonds can be effectively passivated. In addition, parasitic shunts do not occur when negative charges are present at the interface with silicon . Thus, as shown in Figure 6a and Table 1, the photovoltaic parameters of the 4 μm- pitch cell were 0.542 V and 68.1%, respectively, which can be compared with the bulk counterparts. This means that the heterojunction between n-type Si and p-type PEDOT: PSS acts as an excellent rectifying junction, and the Al2O3 layer also efficiently passivates silicon
surface defects. As the pitch of SiMW increased, the Jsc of TSC decreased, which can be explained by the decrease in light absorption. As the pitch increased from 4 μm to 7 μm, the average light absorption of TSC decreased from 78.11 to 38.71% at a wavelength of 400-1100 nm (Table 2). This is in good agreement with the reduction in Jsc. Similar to the change in Jsc, Voc is also inversely proportional to the light transmittance since the Voc of a conventional solar cell is related to photocurrent (IL) and saturation current (I0) as follows: Voc to ln (for IL / optical transparency) Due to the dependence of Voc and Jsc, the efficiency of TSCs also has a trade off with optical transparency, which is inevitable in TSCs.
Nanowire arrays are known to have excellent anti-reflective properties due to graded refractive index effects and light trapping [45-48]. Thus, nanowire arrays can have lower reflectance than microwire arrays. However, nanowire arrays are made by top-down methods [49-51] that include electron beam lithography and subsequently by etching or bottom-up methods [52-54]
that include vapor-liquid-solid methods. Both have very limited scalability of the whole area.
Moreover, these arrays have a very high surface-to-volume ratio, which increases the likelihood of surface recombination and degrades performance. [38, 55, 56]. In contrast, wafer scale microwire arrays are manufactured by widely used photolithography and etching processes. In the semiconductor industry. In addition, microwire arrays are advantageous for forming effective junctions and are easy to collect carriers [37, 57]. Thus, SiMW with reduced reflectance could be a promising candidate for TSC. Assuming that the reflectance of SiMW is proportional to the area of the upper flat surface of the microwire array, the average calculated reflectance obtained with SiMW with a pitch of 4 μm is as high as 9.54% (Figure 8a). Thus, to reduce high reflectance from flat SiMW tips, antireflective (AR) coating or surface texturing techniques typically employed in bulk silicon solar cells can be applied.
First, a TSC with a 70 nm thick SiN AR coating on a SiMW tip deposited by plasma enhanced chemical vapor deposition (PECVD) was prepared. Figure 8b shows the J-V characteristics of a TSC based on a 4μm pitch SiMW array using SiNx. With the use of antireflective films, Jsc increased from 17.07 to 18.94 mA cm[-2], but Voc and FF decreased simultaneously, which did not significantly improve efficiency compared to TSC without a SiN layer. The reduction in Voc can be due to the fact that n-Si and p- PEDOT heterojunctions are formed only on the side, not on the top surface of SiMW, which do not efficiently separate the electron-hole pairs. Thus, an attempt was made to reduce light reflection by changing the shape of the flat SiMW tip (Figure 9a). For this
purpose, a 70 nm thick SiO2 thin film was formed on the tip of the SiMW as an etching mask, and the SiMW was chemically etched using a hydrofluoric acid-nitric acid-acetic acid (HNA) mixed solution [58-61]. Silicon etching with HNA solution proceeds in three steps:
Si + 2H+ → 2Si2+ + H2 (1)
Si2+ + 2OH- → Si(OH)2 → SiO2 + H2 (2)
SiO2 + 6HF → H2SiF6 (3)
The overall reaction is initiated by breaking the covalent bond between silicon atoms by H + ions supplied from HNO3 to produce SiO2 by recombination of Si 2 + ions and hydroxide ions. HF then dissolves the silicon dioxide to produce an aqueous salt.
CH3COOH, on the other hand, acts as a diluent to prevent excessive dissociation of HNO3 and to adjust the etch rate and roughness of the etched surface. SiMPF was intensely etched and even partially removed from the PDMS matrix in the HNA solution with a composition of 3: 7: 0, but the etch rate was significantly attenuated in the HNA etch solution with the 3: 6: 1 composition (Figure 10a and b). However, SiMW is still etched extensively by solution leaving only the Al2O3 layer. In order to reduce the etch rate and change the behavior of HF-based etching, various additives, including organics, have been introduced into HF solutions [61, 62]. Surprisingly, the etching rate was greatly reduced by the etching solution with DMF added instead of acetic acid. And this dramatically changed the shape of the SiMW tip (Figure 10c). Interactions between HF and DMF molecules form heterogeneous bonds. This hetero bond has a pyramidal molecular structure consisting of three H-F bonds (H on DMF and F on HF), which causes redistribution of the electron density of HF, which greatly reduces the etching rate of SiO2. As a result, the etching rate of the native oxide (etching intermediate) as well as the etch oxide of the SiO2 etch mask layer on the top surface of the SiMW is significantly reduced, maintaining the shape of the SiMW tip while maintaining the overall shape of the SiMW. In addition, a series of etching experiments were carried out with varying volume ratios of HF-HNO3- CH3COOH-DMF (HNAD) etching solution and found that HNAD solutions with volume
ratios of 30: 60: 3: 7 produce SiMW well. Defined and uniform inclined tip as shown in Figure 9b. The measured angle of the inclined SiMW tip was ˜54.7 mm3. Simulation of the angle dependent reflection of the inclined tip also shows that the reflectance reaches saturation after decreasing to 45 ° (Figure 9c). Finite differential time domain (FDTD) simulations were performed to study the reflection and absorption of light from planar and slanted SiMW tips.
About 40% of visible and infrared light was reflected back from SiMPF with flat tips; Therefore, the intensity of the electric field inside the SiMW was low (Figure 9d). On the other hand, the light incident on the inclined tip of the SiMW is reflected back toward the inside of the SiMPF and eventually reabsorbed by the adjacent SiMW to increase the intensity of the electric field inside the SiMW. In addition, the low reflectance of the inclined tip SiMPF is mainly due to the reabsorption of light reflected from the inclined tip by the adjacent microwires (Figure 9e).
The time difference between the two absorption events provides evidence that the light reflected from the slope Mw is reabsorbed in the adjacent Si Mw. After 10.5 fs, the electromagnetic energy inside Si Mw increases again, indicating that the reflected light propagates to adjacent Si Mw for 10.5 fs. When multiplied by the group velocity of their pulses 64, it corresponds to 3.17um. This is in good agreement with the distance between the center of the Si MW and the edge side of the adjacent Si MW, indicating that the light reflected from the slanted tip is absorbed back into the adjacent wire (Figure 9f). Thus, the absorbed electromagnetic energy of the inclined microwire consists of the electric field of the first unreflected light (white arrow, figure 9d) and the scattered electric field of red-absorbed light of the refracted light (red arrow, figure 9e). 2G-i show the reflection, transmission and absorption spectra of SiMPF with flat and inclined tips as a function of pitch obtained by UV- Vis spectroscopy measurements. As expected, the average reflectance sharply decreased from 10.48-13.90% for flat SiMPF to 1.81-3.45% for tilted counterparts (Table 3). In particular, flat SiMPFs with a pitch of 4 μm or the highest density of microwires had the lowest reflectance.
This can be explained by the effect of light trapping by scattering and diffraction due to the narrow spacing (~ 2 μm) between the Si MW [65, 66]. The transmission spectra of planar and slanted SiMPF were determined mainly by pitch, and were similar except that the transmittance of the slanted wavelength was slightly lower than that of the planar sample in the long wavelength region. The extinction coefficient of silicon is small due to the indirect band gap structure and tends to decrease exponentially with increasing wavelengths [67, 68]. Thus, the 30 μm thick silicon layer used in this study may not fully absorb 1- illumination. 69. To determine the origin of this difference in the transmittances of flat and sloped samples, a time-
resolved light tracking simulation was performed. It was performed at two wavelengths (short:
550nm) and (long: 900nm). For short wavelength incident light, the light intensity rapidly attenuates as the depth of the microwire increases for both flat and slanted samples, indicating that the short wavelength light is fully absorbed by 30 μm thick Si (Figures 11a and b). . On the other hand, in the case of having long wavelength incident light on a flat SiMW, the light absorption was so weak that a substantial portion of the light was transmitted through the bottom of the SiMW (Figure 12a). However, when long wavelength light was incident on the inclined tip having an incident angle of 50 °, the light was refracted at the air-silicon interface so that the light inside the microwire followed the zigzag path (Figure 12b). Increase the effective light path or decrease the transmittance (Figure 9h). As a result, the absorption calculated from the reflection and transmittance data was significantly improved in the gradient SiMPF (Figure 9I). For example, absorption in SiMW with a pitch of 5 μm increased from 59.24% for flat samples to 72.80% (increasing 13.56%) for tilted relative. Average reflectance, transmittance and absorption of the flat and sloped SiMPFs are summarized in Tables 2 and 3.
When applying TSC, the haze value is important. This is because the haze value can reduce the sharpness when viewing something. Haze values represent light scattering and were calculated using the following equation:
Haze (%) = T_ Diffusion / T_ Total
Where T total is total transmittance and T diffuse is diffuse transmittance (detailed measurement methods and additional information in Figure 13) [70, 71]. As expected, the narrower the pitch between the microwires, the higher the actual scattering. Thus, samples with tighter pitches showed higher haze ratios. At a narrow pitch of 4um, haze values greater than 15% are relatively high. On the other hand, a sample with 7um pitch shows very low haze of ~ 2.5%, which can also be compared with ultra-thin silver nanowires with indium tin oxide or haze varieties of 1-3% (Figure S14a) [72-74] . Interestingly, the denser the pitch, the larger the haze ratio difference between flat and sloped. The inclined tip of the microwire causes the light inside the microwire to follow the zigzag path (path "A" in Figure 14b) or reflect back toward the adjacent microwire (path "B" in Figure 14b). Light along the path "A" is almost absorbed.
On the other hand, the light of path "B" causes a second scattering into adjacent Si, so that the
haze can be increased for a particularly dense pitch of the sample. Figure 15a is an optical photograph showing the neutral color perception of SiMPF with controlled pitch, unlike perovskite filters. Samples with pitches of 7 um (I), 6 um (II), 5 um (III) and 4 um (IV) were displayed on the college logo background. Transparency changed according to pitch, but color was recognized without distortion. For accurate evaluation of color recognition, SiMPF was illuminated with simulated AM1.5 light, and the color coordinates of the transmitted light are shown in the CIE 1931 chromaticity diagram as shown in Figure 15b and Table 4. The color coordinates of the various dyes commonly used for dye-sensitized solar cells (DSSC) and MAPbIxBr3xx perovskite films are also shown. In this study, perovskite thin films were prepared and dye data for DSSC were referenced in other publications [16, 75, 76]. The dye is green or blue tint and the perovskite film is reddish brown to yellow (Figure 16, SiMPF in this study has chromaticity coordinates in the central region of the chromaticity diagram). Figure 15c shows the IV characteristics of a TSC using tilted SiMPF, and detailed photovoltaic power performance is summarized in Table 5. Since HNAD etching only affects the top of the already exposed Si microwires in the first step, they still exist regardless of the flat and tilted tip of the Al2O3 passivation microwire array on the side. Thus, compared to TSC based on flat SiMPF, the Voc and FF of the tilting device remained unchanged, while the Jsc increased significantly. In addition, manufacturing processes involving HNAD etching are still reproducible. As shown in Figure 17, the box plot of the photovoltaic parameters of the slanted SiMPF also has a narrow distribution.
Interestingly, the improvement in Jsc (ΔJsc) increased as the pitch of SiMPF increased, which is in good agreement with the change in light absorption as a function of the pitch of the flat sloped sample. TSCs with a pitch of 4 μm showed the highest efficiency of 8.07%. Figure 15d shows the EQE spectrum of a gradient TSC with a different pitch of 4-7 μm in the wavelength range of 400-1100 nm. Integrated Jsc matches that determined from the J-V curve. Comparing the EQE of the flat and sloped samples showed a significant increase in the current density of the sloped sample in the near-infrared region rather than in the visible region (Figure 18). In other words, improving the efficiency of TSCs is achieved by improving absorption in the near infrared region (800- 1100 nm) without compromising visible transparency, one of the main parameters of TSCs. Figure 15e shows a plot of the efficiency versus average transmittance of visible light in various neutral colored transparent solar cells, including those based on perovskite, organic semiconductors, and amorphous silicon. Zhang et al. Taking
advantage of the NIR non fullerene receptor at a light transmittance of 20% , it demonstrated ~ 9% neutral color TSC. Chueh et al. By reducing the thickness of the light absorbing layer and the silver electrode in the organic solar cell was prepared TSC with an efficiency of 5.63% at a light transmittance of 13%. Yi et al. Metal electrodes were replaced with graphene electrodes, showing a transparent organic solar cell that achieved an efficiency of 3.8% at 79% with transparent visibility. Eperon et al.
Introduced a microstructured perovskite and enabled the transmission of light through the device, achieving an efficiency of ~ 7% at visible transparency of 8%.
Alternatively, even when a thin layer of a-Si (<300 nm) was used for the active layer of TSCs , the adjustable transparency range was very limited. As the transmittance increases, an uncontrolled shunt path is formed into thin a-Si, which results in a significant loss of efficiency, further worsening the transmittance gain. Overall performance is comparable to the latest TSCs based on organic or perovskite, but slightly lower in transparency compared to TSC (T> 30%) with high transmission. To improve transparency, the surface treatment of PDMS that fills the spaces between the microwires can be further considered for future work. However, the transparency of the device based on the SiMPF platform can be easily adjusted from 10% to 55% by changing the gap between Si MWs, unlike other developed TSCs. More importantly, SiMPF-based TSCs can be applied as flexible solar cells due to the thinness of the device and the inherent robustness of PDMS [82-84], while most of the currently reported TSCs using organics or perovskite are rigid without flexibility. Glass.
TSCs are characterized after bending and periodic bending tests. Interestingly, the performance of transparent solar cells consisting of PEDOT: PSS / Si Mw – PDMS composites / IZO does not significantly decrease in the bending state of 12 mm and 6 mm bend radii (Figures 19a and 19b). Photonic parameters of the device in the bent state are summarized in Table 6. In addition, as shown in Figure 19c, after a cyclic bending test with a bending radius of 6 mm, the normalized efficiency is maintained almost without a significant decrease, which can cause the transparent solar cell to bend. In addition, since SiMPF was manufactured using large area processes such as photolithography and dry etching, it can be easily scaled to wafer scale, unlike perovskite and organics, as shown in Figure 19d and 19e. As shown in Figure 20a, the optical diffraction pattern is generated by transmitted light and exhibits Fourier transform properties between the domains. Even after applying 50% strain, a long-range sequence, still representing the cross-domain of the wire array, was still observed, indicating that the form remains without structural disassembly. After PEDOT: PSS was coated on SiMPF prior to IZO